high heating rate reaction dynamics of al/cuo ... mrz/pdfs/2017_jpc_nanocal.pdf · high heating...
Post on 01-Sep-2018
Embed Size (px)
High Heating Rate Reaction Dynamics of Al/CuO Nanolaminates byNanocalorimetry-Coupled Time-of-Flight Mass SpectrometryJeffery B. DeLisio,, Feng Yi,, David A. LaVan,*, and Michael R. Zachariah*,
Department of Chemistry and Biochemistry, and Department of Chemical and Biomolecular Engineering, University of Maryland,College Park, Maryland 20742, United StatesMaterials Measurement Science Division, Material Measurement Laboratory, National Institute of Standards and Technology,Gaithersburg, Maryland 20899, United States
*S Supporting Information
ABSTRACT: Highly tunable reactive nanolaminates have beenof recent interest for various on chip energetic applications.The reaction dynamics of Al/CuO nanolaminates wereinvestigated by nanocalorimetry-coupled time-of-flight massspectrometry, capable of simultaneous measurement of temporalthermal dynamics and detection of evolved gas phase species atheating rates up to 106 K/s. The nanolaminates weresynthesized by alternately sputtering Al and CuO onto theheater of nanocalorimeter sensors. For thin films of 80 nm withone bilayer, the stoichiometric ratio of fuel to oxidizersignificantly affected the reaction mechanism: initial reactionsoccurred between 300 and 400 C, and main reactions variedbased on stoichiometry. For thicker films of 199 and 266 nm, aseries of samples with varying bilayer numbers were analyzed todetermine the effect of diffusion distance and interfacial area. Only one reaction step was observed for a sample with a bilayerthickness of 33 nm. A two-step reaction mechanism is observed as the bilayer thickness was increased to 66 nm and beyond:solid-state reaction occurring at the interfaces of Al and CuO before the melting of Al and a much faster liquidsolid reactionright after the melting of Al. At the same time, interfacial premixed distance during the deposition was also estimated fromparallel experiments. Furthermore, the power data from nanocalorimetry provides a more direct method, compared to opticalemission and mass spectrometry based methods, in determining the ignition temperature in addition to being able to measureactual energy output for films with nanoscale thicknesses.
INTRODUCTIONEnergetic nanocomposites have been of recent interest for awide variety of applications due to their high volumetric energydensities, relatively fast reaction kinetics, and decreased ignitiontemperatures.13 The enhancements gained when usingnanosized components, as opposed to micron-sized particles,are due to increased interfacial area and decreased diffusionlength scales. These systems are typically composed of a metalfuel, most commonly aluminum (Al), and a metal oxideoxidizer. Energetic nanocomposites can be manufactured with awide range of architectures ranging from physical mixtures ofnanosized particles to sputter deposited multilayered nanofoils,often referred to as nanolaminates.4,5
Nanolaminates, in particular, have various uses in micro-electromechanical systems (MEMS), microelectronics, andmaterial bonding applications.610 The simple geometry atthe fuel/oxidizer interface of multilayered laminates alsoprovides an ideal system to further study the oxygen transportin thermite based reactions, making it possible to probe factorssuch as the influence of interface-to-volume ratio and its effecton ignition and energy release. These systems can have very
low ignition temperatures (below the melting point of Al) andenhanced reactivity based on the number of bilayers.11,12
The reaction dynamics of energetic nanolaminates have beenextensively studied at relatively slow heating rates (10 K/min)using differential scanning calorimetry and thermogravimetricanalysis.11,13,14 A recent study by Egan et al. used high heatingrate analytics, which more accurately represent the time scalesof a combustion event, to determine the effect of bilayerthickness on the reaction mechanism of Al/CuO nano-laminates.12 Egan et al. used temperature jump (T-jump)time-of-flight mass spectrometry (ToF-MS) coupled with highspeed videography to measure the ignition temperature of 112 bilayer nanolaminates with a fixed total thickness.In this work, the reaction dynamics of the Al/CuO
nanolaminate system was further studied by replacing the T-jump ignition system with a chip based nanocalorimetercapable of collecting thermal data while heating at rates of up to
Received: November 4, 2016Revised: January 5, 2017Published: January 7, 2017
2017 American Chemical Society 2771 DOI: 10.1021/acs.jpcc.6b11114J. Phys. Chem. C 2017, 121, 27712777
106 K/s.15 The integration of nanocalorimetry with ToF-MSallows for simultaneous temporal thermal and speciationmeasurement.16 The incorporation of the nanocalorimeteralso allows for the study of Al/CuO nanolaminates withsignificantly thinner bilayers than those previously studied,which do not visibly show ignition occurring. We report theeffects of stoichiometry, total thickness, and individual bilayerthickness on the reaction mechanism of Al/CuO nanolaminatesin addition to providing a more accurate method to determinethe ignition temperature of these systems.
EXPERIMENTAL SECTIONSample Preparation. The Al/CuO laminates were
prepared using sputter deposition techniques. The Al andCuO sputter targets were purchased from Kurt Lesker, and theCuO target was indium bound to a copper backing plate forbetter heat dissipation during the sputtering. A DC power of300 W is used for aluminum sputtering, and a RF power of 300W is used for CuO sputtering. The sputtering was performedunder a pressure of 0.67 Pa of argon. During deposition, thetarget not in use was turned off to prevent contamination. XRDanalysis (Figure S1) was performed on a sputter deposited pureCuO film to verify the composition. The nanocalorimetersensor has a 100 nm-thick platinum heater suspended on a 100nm-thick silicon nitride membrane in a silicon frame. Thesamples are deposited on the silicon nitride side of thenanocalorimeter sensor. As shown in Figure 1, 10 nm ofalumina was deposited using atomic layer deposition to serve asa barrier layer between the sample and sensor. The first and lastlayer deposited was aluminum so that one bilayer is defined astwo half layers of aluminum and one layer of copper oxide asshown in Figure 1a. Sample thicknesses, bilayer thickness, andstoichiometry of the laminate were varied to investigate thereaction dynamics of Al/CuO nanolaminates.Nanocalorimetry Measurements. The nanocalorimetry
system can measure a thermal signal at heating rates up to 106
K/s. The calibration of the nanocalorimeter sensors used in thiswork has been previously described in detail.17 Briefly, theresistance and temperature were recorded by electricalmeasurements and an optical pyrometer during the resistiveheating/cooling. In order to calculate enthalpy, a previouslypublished method18 was used that entailed heating each emptynanocalorimeter sensor at various heating rates to determinethe heat losses and heat capacity of the bare sensor. The power
associated with the sample could then be calculated from thetotal power by subtracting the power associated with the baresensor and the heat losses. Optical emission from the chipduring heating was also recorded using a high speed camera(Phantom v12.0, 67,000 frames per second), but that data isnot part of the nanocalorimeter measurement.
Time-of-Flight Mass Spectrometer System. A previ-ously reported technique describes the integration of thenanocalorimeter into a time-of-flight mass spectrometer (ToF-MS).16 Figure 1b shows a diagram of the integrated setup withhigh speed videography to record optical emission fromreaction. Specific details of the linear ToF-MS system usedfor this study have been previously reported.19,20 Thenanocalorimeter sensor was inserted into the ionization regionof the ToF-MS using a linear motion feedthrough with a 3Dprinted adapter and sensor cover. A sampling rate of 100 s perspectrum (10 kHz) was used to capture the progress of thereaction with 100 spectra obtained post-triggering for each run.Gas phase reaction products were ionized for 3 s using anelectron gun operated at 70 eV and 1 mA. The data wascaptured and processed using a 600 MHz digital oscilloscope.
RESULTSEffect of Stoichiometry on Al/CuO Reaction. In order
to first evaluate the effect of stoichiometry on the reactionmechanism, films of varying equivalence ratios () were rapidlyheated on the nanocalorimeter within the ionization region ofthe ToF-MS. Figure 2 shows the nanocalorimetry results fromrapid heating (105 K/s) of the respective Al/CuO nano-laminates. These samples each have only one bilayer. The ratioof Al:CuO was varied, and the total thickness was kept constantat 80 nm. All three samples show an initial exothermic peakwith an onset temperature between 300 and 400 C. Thethermal data was much clearer for the fuel-rich sample with thepredominant exotherm occurring at the melting point of Al.The third exothermic reaction occurred around the decom-position temperature of CuO. This sample was run a secondtime (Figure S2), and a sharp endotherm was detectedcorresponding to the AlCu eutectic. As the equivalenceratio reduced to 1, the stoichiometric ratio, the main reactionexotherm was shifted to a higher temperature closer to thedecomposition of CuO. This may be related to the diffusivity ofliquid aluminum. The main exothermic peak becomes muchbroader in the fuel-lean sample and spans from the melting
Figure 1. Diagram of sputter deposited single bilayer Al/CuO nanolaminate (a) and ToF-MS experimental setup with integrated nanocalorimeterand high speed imaging (b).
The Journal of Physical Chemistry C Article
DOI: 10.1021/acs.jpcc.6b11114J. Phys. Chem. C 2017, 121, 27712777